Piezochromic Porous Metal-Organic Framework.
Andrzejewski, Michał; Katrusiak, Andrzej; The journal of physical chemistry letters 8 (2017) 279–284; doi:10.1021/acs.jpclett.6b02458

data_8000382
_publ_section_title
;
 Piezochromic Porous Metal-Organic Framework.
;
_journal_issue                   1
_journal_name_full               'The journal of physical chemistry letters'
_journal_page_first              279
_journal_page_last               284
_journal_paper_doi               10.1021/acs.jpclett.6b02458
_journal_volume                  8
_journal_year                    2017
_chemical_formula_moiety         'C14 H18 Co N2 O5'
_chemical_formula_sum            'C14 H18 Co N2 O5'
_chemical_formula_weight         353.23
_chemical_name_common            AMU1
_chemical_name_systematic
;
Co(1,4-benzenedicarboxylate)(1,4-diazabicyclo[2.2.2]octane)H2O
;
_space_group_crystal_system      triclinic
_space_group_IT_number           1
_space_group_name_Hall           'P 1'
_space_group_name_H-M_alt        'P 1'
_atom_sites_solution_hydrogens   mixed
_atom_sites_solution_primary     direct
_audit_creation_date             2016-07-12
_audit_creation_method
;
Olex2 1.2
(compiled 2016.02.19 svn.r3266 for OlexSys, GUI svn.r5155)
;
_cell_angle_alpha                89.95(3)
_cell_angle_beta                 97.84(4)
_cell_angle_gamma                94.966(12)
_cell_formula_units_Z            1
_cell_length_a                   5.7216(11)
_cell_length_b                   6.9763(8)
_cell_length_c                   10.501(12)
_cell_measurement_reflns_used    732
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      52.894
_cell_measurement_theta_min      9.342
_cell_volume                     413.7(5)
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXS (Sheldrick, 2008)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.234
_diffrn_measured_fraction_theta_max 0.225
_diffrn_measurement_device_type  'multiwire proportional'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1708
_diffrn_reflns_av_unetI/netI     0.1446
_diffrn_reflns_Laue_measured_fraction_full 0.234
_diffrn_reflns_Laue_measured_fraction_max 0.225
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       4
_diffrn_reflns_limit_l_min       -3
_diffrn_reflns_number            1759
_diffrn_reflns_point_group_measured_fraction_full 0.234
_diffrn_reflns_point_group_measured_fraction_max 0.225
_diffrn_reflns_theta_full        26.000
_diffrn_reflns_theta_max         26.447
_diffrn_reflns_theta_min         4.671
_exptl_absorpt_coefficient_mu    1.060
_exptl_absorpt_correction_T_max  0.909
_exptl_absorpt_correction_T_min  0.892
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
Data were collected and reduced by program CrysAlisPro, 
and SCALE3 ABSPACK was used for absorption correction
;
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    1.418
_exptl_crystal_description       plate
_exptl_crystal_F_000             183
_exptl_crystal_size_max          0.3
_exptl_crystal_size_mid          0.1
_exptl_crystal_size_min          0.1
_refine_diff_density_max         1.518
_refine_diff_density_min         -1.011
_refine_diff_density_rms         0.297
_refine_ls_abs_structure_details
;
 Refined as a perfect inversion twin.
;
_refine_ls_abs_structure_Flack   0.5
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   2.268
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     59
_refine_ls_number_reflns         732
_refine_ls_number_restraints     46
_refine_ls_restrained_S_all      3.721
_refine_ls_R_factor_all          0.2971
_refine_ls_R_factor_gt           0.2433
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.2000P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.5368
_refine_ls_wR_factor_ref         0.5804
_reflns_Friedel_coverage         1.000
_reflns_Friedel_fraction_full    0.234
_reflns_Friedel_fraction_max     0.225
_reflns_number_gt                489
_reflns_number_total             732
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            jz6b02458_si_004.cif
_cod_data_source_block           203GPa_P1
_cod_database_code               8000382
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups, All C(H,H) groups
 At 1.5 times of:
  All O(H) groups
2. Restrained distances
 C8-C1
 1.48 with sigma of 0.002
 C4-C3
 1.36 with sigma of 0.002
 C3-C2
 1.36 with sigma of 0.002
 C2-C1
 1.36 with sigma of 0.002
 C1-C6
 1.36 with sigma of 0.002
 C6-C5
 1.36 with sigma of 0.002
 C5-C4
 1.36 with sigma of 0.002
 N1-C9
 1.48 with sigma of 0.002
 N1-C13
 1.48 with sigma of 0.002
 N1-C11
 1.48 with sigma of 0.002
 C10-N2
 1.48 with sigma of 0.002
 C12-N2
 1.48 with sigma of 0.002
 N2-C14
 1.48 with sigma of 0.002
 C14-C13
 1.52 with sigma of 0.002
 C10-C9
 1.52 with sigma of 0.002
 C12-C11
 1.52 with sigma of 0.002
 O3-C7
 1.23 with sigma of 0.002
 O2-C8
 1.23 with sigma of 0.002
 C4-C7
 1.34 with sigma of 0.002
 O1_$2-Co01
 2.1 with sigma of 0.02
 O1-O2
 2.16 with sigma of 0.002
 C10-C12
 2.5 with sigma of 0.02
 O4-O3
 2.16 with sigma of 0.02
 O1W-O4
 2.7 with sigma of 0.02
 O1W_$3-O2_$4
 2.1 with sigma of 0.02
 C2-C8 \\sim C8-C6
 with sigma of 0.02
 O4-C4 \\sim C4-O3
 with sigma of 0.02
 O4-Co01 \\sim Co01-O3
 with sigma of 0.02
 C5-C7 \\sim C7-C3
 with sigma of 0.02
 O1-C1 \\sim C1-O2
 with sigma of 0.02
 O1-C1 \\sim C1-O2
 with sigma of 0.02
3. Restrained planarity
 C8, C6, C1, C2, C3, C4, C5
 with sigma of 0.1
 C8, C6, C1, C2, C3, C4, C5, C7, O4, O3, O2, O1
 with sigma of 0.1
4. Uiso/Uaniso restraints and constraints
Uiso(C4) = Uiso(C5) = Uiso(C3) = Uiso(C2) = Uiso(C1) = Uiso(C6) = Uiso(C8)
Uiso(O3) = Uiso(O4)
Uiso(N1) = Uiso(N2) = Uiso(C9) = Uiso(C12) = Uiso(C14) = Uiso(C10) = Uiso(C13)
= Uiso(C11)
Uiso(O1) = Uiso(O2) = Uiso(O3) = Uiso(O4)
Uiso(C6) = Uiso(C1) = Uiso(C2) = Uiso(C3) = Uiso(C4) = Uiso(C5) = Uiso(C8) =
Uiso(C7)
5. Others
 Fixed Uiso: O1W(0.0241)
 Fixed X: H1WA(0.39922) H1WB(0.49922)
 Fixed Y: H1WA(-0.053541) H1WB(-0.053541)
 Fixed Z: H1WA(-0.06268) H1WB(0.07268)
6.a Secondary CH2 refined with riding coordinates:
 C11(H11A,H11B), C9(H9A,H9B), C12(H12A,H12B), C14(H14A,H14B), C10(H10A,H10B),
 C13(H13A,H13B)
6.b Aromatic/amide H refined with riding coordinates:
 C6(H6), C2(H2), C3(H3), C5(H5)
6.c Fitted hexagon refined as free rotating group:
 C6(C1,C2,C3,C4,C5)
;
_shelx_hkl_checksum              59843
_olex2_submission_special_instructions 'No special instructions were received'